IOSR Journal of Electrical and Electronics Engineering (IOSR-JEEE) e-ISSN: 2278-1676,p-ISSN: 2320-3331, Volume 6, Issue 6 (Jul. - Aug. 2013), PP 79-83 www.iosrjournals.org
Controlling Charge Injection in Organic Field-Effect Transistors Using Self-Assembled Monolayers M. K. Madhu1, Dr. D. Chandra Sekhar Reddy2 Abstract: We have studied charge injection across the metal/organic semiconductor interface in bottomcontact poly (3-hexylthiophene) (P3HT) field-effect transistors, with Au source and drain electrodes modified by selfassembled monolayers (SAMs) prior to active polymer deposition. By using the SAM to engineer the effective Au work function, we markedly affect the charge injection process. We systematically examine the contact resistivity and intrinsic channel mobility, and show that chemically increasing the injecting electrode work function significantly improves hole injection relative to untreated Au electrodes.
Improved understanding of the dynamics of charge motion at interfaces between metals and organic semiconductors (OSCs) is crucial for optimizing the performance of organic optoelectronic devices, including organic field-effect transistors (OFETs). In an OFET the electronic structure of the OSC/contacting electrode interface can strongly affect the overall performance of the device. The band alignment at the OSC/metal interface is influenced by several factors such as interfacial dipole formation [1, 2, and 3], electrode contamination , and OSC doping [5, 6, and 7]. Depending on the particular band alignment, the charge injection mechanism can significantly change, as seen by e.g. linear (ohmic) or nonlinear current-voltage characteristics. Ohmic contacts between metals and inorganic semiconductors are often achieved by strong local doping of the contact regions, but such an approach is challenging to implement in OSCs. Bulk doping levels in the OSC do affect injection. In recent work  examining charge injection in bottom-contact OFETs based on poly(3-hexylthiophene) (P3HT), we found that large contact resistances and nonlinear transport at low dopant concentrations are consistent with the formation of an increased injection barrier for holes. Band alignment is also significant . For example , the onset of nonohmic transport at low doping is much more severe in devices with Au source and drain electrodes than Pt. It has previously been shown[9, 10, 11, 12] that, by self assembly of a layer of molecules with an intrinsic electric dipole moment, the work function of metal electrodes can be lowered or raised, affecting the size of the injection barrier at the metal/OSC interface. While limited attempts have been made to use this approach to engineer contacts in OFETs [13, 14], considerably more effort has been dedicated to contacts in organic light emitting diodes (OLEDs)[10, 11, 17] and modification of the OSC/dielectric interface[15, 16] in OFETs. In contrast to OLEDs, OFETs allow studies of transport with a single carrier type, with carrier density tunable independently of the source-drain bias, and with established procedures for discerning between contact and bulk effects. Minimizing contact resistances is particularly challenging in planar OFETs since active contact areas are generally much smaller than in vertical OLEDs.
In this work, using channels of varying length, we systematically examine the contact resistances and true channel mobility at various doping levels of bottomcontact P3HT OFETs with Au electrodes modified by self-assembly of dipolar molecular monolayers. We correlate the transport data with self-assembled monolayer (SAM) induced work function changes as measured by scanning potentiometry. In the case of electron-poor (work function-raising) SAMs, we show that contact resistances remain low compared to the channel resistance and the transistors show linear transport. These observations are consistent with the “pinning” of the local chemical potential at the interface at an energy favorable to hole injection, and contrast sharply with the strongly nonlinear injection observed at low doping levels in OFETs made with bare Au electrodes. Furthermore, devices with electrodes modified by electron rich (work function-lowering) SAMs show nonlinear transport and low currents at all doping levels, becoming increasingly nonlinear as dopant density is reduced. This is consistent with formation of an increased injection barrier for holes in such devices. OFETs are made in a bottom-contact configuration  on a degenerately doped p+ silicon wafer used as a gate. The gate dielectric is 200 nm of thermal SiO2. Source and drain electrodes are patterned using electron beam lithography in the form of an interdigitated set of electrodes with systematic increase in the distance between each pair. The channel width, W, is kept fixed for all devices at 200 μm. The electrodes are deposited by electron beam evaporation of 2.5 nm of Ti and 25 nm of Au, followed by lift off. This thickness of metal is sufficient to guarantee film continuity and www.iosrjournals.org
79 | Page
Controlling Charge Injection In Organic Field-Effect Transistors Using Self-Assembled Monolayers good metallic conduction while attempting to minimize disruptions of the surface topography that could adversely affect polymer morphology. Prior to SAM assembly, the substrates were cleaned for 2 min in oxygen plasma. They were then immersed cumulation mode. With the source electrode grounded, the devices are measured in the shallow channel regime (VD < VG). Figure 1(a) shows the transport characteristics of a Au/P3HT device with L = 40 μm at T = 300 K and at a fixed VG = −70 V for different doping levels. In anneal1, the sample was vacuum treated in the analysis chamber at 300 K for 16 h. Anneal2 corresponds to the sample being further heated in vacuum for 18 h at 350 K, while anneal3 includes yet an additional 18 h at 360 K. As in earlier experiments , the transport in this device with unmodified Au electrodes becomes nonlinear at high annealing steps and the current drops by orders of magnitude. We attributed this to the formation of an increased injection barrier for holes, and similar effects have been reported by others .
Results And Discussion
Figure 1a shows the transport characteristics of an Au/P3HT device with L = 40 μm at T = 300 K and at a fixed VG = −70 V for different doping levels. In anneal1, the sample was vacuum treated in the analysis chamber at 300 K for 16 h. Anneal2 corresponds to the sample being further heated in vacuum for 18 h at 350 K, while anneal3 includes yet an additional 18 h at 360 K. As in earlier experiments described in Chapter 4, the transport in this device with unmodified Au electrodes becomes nonlinear at high annealing steps, and the current drops by orders of magnitude. We attributed this to the formation of an increased injection barrier for holes, and similar effects have been reported by others .
Figure.1: a) A log-log plot of the transport characteristics of a Au/P3HT device for different annealing as described in the text. b) Similar plot for a Au/P3HT device with the electrodes modified by F-OPE SAM shown in the inset. (c) Au/P3HT device with electrodes modified by OPE-NH2 SAM molecules shown in the inset. For all devices, L = 40 μm at T = 300 K and at a fixed VG = −70 V with the same annealing schedule. The solid black line has a slope of 1. In contrast, Fig.1b shows the transport for a device with similar geometric parameters and annealing schedule, in which the electrodes were modified by F-OPE SAM molecules prior to P3HT deposition. Even though ID drops at higher annealing steps, the currents remain linear with VD and as shown below, the contact resistance remains much lower compared to bare Au devices. This behavior is similar to our previous observations for Pt/P3HT devices. These effects have been verified in annealing cycles on multiple arrays of FOPE treated devices. In Fig.1c, the electrode surfaces were modified by OPE-NH2. In this case, the currents are much lower than in either (a) or (b), and even when the hole doping of the P3HT is significant, injection is non-Ohmic, with ID rising super-linearly with VD. In highly annealed conditions, this behavior is super-quadratic. Transport data for the OPE-2(NH2) treated devices qualitatively looks very similar to those in Fig.1c. From the data in Figs.1a and 1b, we extract the channel resistance, Rch, the intrinsic device mobility, μ, and the contact resistance Rs from the L dependence of the total device resistance, Ron ´ ∂VD/∂ID over a T and VG range as described in section 3.2. We obtain Rs in the limit |VD| < 1V, where transport is still reasonably linear even after the longer annealing runs. We note that while we have developed a procedure for extracting contact current-voltage characteristics even in the limit of strong injection nonlinearities (section 3.3), it is difficult to quantify such www.iosrjournals.org
80 | Page
Controlling Charge Injection In Organic Field-Effect Transistors Using Self-Assembled Monolayers injection by a single number such as Rs. In the shallow channel limit, it is straightforward to convert the gate dependence of Rch into field-effect mobility. Figure 2 shows a log-log plot of μ vs Rs for two sets of devices over a series of temperatures and gate voltages for an initial annealing step. The open symbols correspond to data from the F-OPE treated electrodes and the filled symbols are extracted from bare Au/P3HT data. The error bars come from the uncertainty in the slope and intercept of Ron vs. L plots. Indeed, in device arrays with Rs << Rch, deviations from perfect scaling of Rch / L can lead to “best fit” values of Rs that are actually negative (and hence cannot be plotted on such a figure), though with appropriately large error bars. Here, the mobility and the contact resistance for both device sets are similar, consistent with similarity in the magnitude of ID − VD for both samples. In the proceeding annealing steps, however, the contact resistance for the sample with untreated electrodes increases significantly, compared to the SAM treated device (Figs.2b and (c)). Whereas the Au/P3HT devices become severely contact limited at high dedopings, the treatment of Au electrodes with F-OPE molecules keeps the contact resistance relatively low compared to channel resistance, and the transport characteristics remain linear. This Ohmic injection persists even when bulk VG = 0 conduction in the P3HT film is completely suppressed at room temperature. Our results in F-OPE treated devices are quantitatively similar to those obtained in charge injection from Pt electrodes into P3HT as outlined in Chapter 4. Although it is difficult to probe the energy level alignment directly at the metal/organic interface (due to the thick P3HT film resulting from solution casting), it is clear that increasing the Au effective work function results in improved electronic performance of these OFETs. In light of the many experiments showing the formation of interfacial dipoles at the metal/OSC interface upon deposition of the OSC [67, 70, 71], it is possible that introduction of work function-raising SAMs such as F-OPE in our experiments counteracts or prevents the work function-lowering effect of these interfacial dipoles.
Figure 2: a) A log-log plot of μ vs Rs for 2 sets of devices over a series of tempera-tures and gate voltages. The open symbols correspond to data from the F-OPE treated electrodes and the filled symbols are extracted from bare Au/P3HT data. Anneal1 here corresponds to sample being pumped on in vacuum at 320 K overnight. b) Data retaken after sampled was annealed at 350 K for 18 h (anneal2). c) Data taken again after another anneal step similar to (b). The reason for fewer data points in parts (b) and (c) for SAM treated sample is a smaller contact resistance with significant error compared to the channel resistance. Pinning of the energy levels at the interface such that there is a small or non-existent injection barrier for holes. On the other hand, the work functionlowering OPE-NH2 SAMs appear to contribute more substantially to the interfacial dipoles, resulting in significant Schottky barrier formation for holes at the interface and severe nonlinear injection in these devices. The subsequent dedopings have the same implications. One must also consider whether the different injection properties could result from SAM-induced changes in the ordering of the P3HT at the metal-OSC interface. Such morphological differences may occur, and would require careful interface-sensitive spectroscopes or scattering measurements to confirm. However, while improved P3HT ordering at the F-OPE/P3HT interface would result in higher mobilities and lower contact resistances, we find it unlikely that morphological changes alone could explain the dramatic difference in injection properties as a function of doping. The data in Fig.2 strongly suggest significant differences in the band energetic between the F-OPE treated and untreated Au electrodes.
81 | Page
Controlling Charge Injection In Organic Field-Effect Transistors Using Self-Assembled Monolayers IV.
Conclusion And Future Scope
We have used dipole-containing self-assembled monolayers on the Au source and drain electrodes to strongly manipulate the charge injection process across the metal-organic interface in a series of polymer FETs based on P3HT. To see the effect of dopant concentration on device performance, we measure device properties after each of a series of mild annealing steps in vacuum. We extract the contact resistances and the intrinsic channel mobility from the length dependence of the resistance for bare Au/P3HT and flourinated-OPE Au/P3HT devices where transport is still relatively linear at low drain bias. At low dopant concentrations, SAM-modified devices show significantly lower contact resistances and higher mobilities compared to unmodified devices. We attribute these findings to higher metal work function and small injection barriers for holes in the case of F-OPE SAM modified devices, resulting from better energetic alignment with the valence band of the organic semiconductor. These results quantitatively demonstrate the power of simple surface chemistry in modifying the dynamics of charge at interfaces with OSCs, even in nearly undoped material. Such techniques will be generally useful in significantly improving technologies based on these versatile materials. In this work, we investigated a series of outstanding problems related to charge injection and transport in organic field-effect transistors. This is a relatively new area and more work needs to be done in way of understanding the nature of charge transport in these devices. I am very honored and pleased to have contributed to the growth of this field through our experiments and analyses and under the guidance of my advisor and by many contributions from our collaborators. Our results of linear charge injection from Au electrodes into P3HT, for example, demonstrated that contact resistivity and the true channel mobility are closely related and models of charge injection should address this relationship. For the nonlinear data analysis from metals with low work functions, we developed a technique of extracting the contact current-voltage characteristics from the transport data by using the scaling of the current with channel length. This data was then compared with the predictions of a recent hopping injection model with emphasis on the primary injection event. We showed that an energy-dependent disordered density of localized states in the organic semiconductor seems to be an important factor for the weak temperature dependence of the currents observed in our transistor devices. This indicates that diffusion-limited models are not entirely reliable. However, there are several unaddressed issues in our analysis of the nonlinear data. The most interesting is the presence of small depletion regions formed in the vicinity of the contacts. The size of this region, the charge carrier density and mobility and the gate voltage dependence of the current are all important issues that need to be investigated in detail. Improved local probes, such as high resolution scanning potentiometry or scanning tunneling microscopy, would be extremely useful in better understanding these depletion regions. Also, more theoretical work and modeling on the nature of these regions are essential. One experiment that can be performed here at Rice as a continuation of this work is fabrication of small gaps on the order of 100 nm and below followed by extensive measurements of device characteristics as a function of temperature and the gate voltage. At such length scales, the transistor channel made from low work function contact metals is expected to comprise partially or entirely of a depletion region. By fabricating devices with various metals and measuring the transport at different annealing steps, we expect to gain valuable information about the operation of the device in this regime. The ultimate goal of this proposed experiment, however, is to fabricate devices with small enough gaps (âˆź 10 nm) that could allow us to measure transport through single polymer chains. In this case, the charge carriers should move along the polymer chain and not be limited by inter-chain hopping. Therefore, we expect to observe a bandlike transport. The mobility should remain the same or even improve, as temperature is lowered. This is a complete diversion from the current trend in almost all organic semiconducting devices and has the potential to be a ground-breaking work. Fabricating nanogaps also allows for transport studies in the regime of extremely high electric fields without using high operating voltages. In light of a recent work , suggesting voltage-induced metal-insulator transition in polythiophene transistors at high gate and source-drain voltages, this can be an interesting experiment to examine whether this is a result of a true transition or is simply due to a temperature-independent process such as tunneling of carriers between localized states. We also performed several experiments investigating the influence of dopants and work function fluctuations (through self-assembly of monolayers) on band alignment at the metal/organic semiconductor interface. The doping experiments revealed that at lower dopant concentrations, the size of the hole injection barrier between the organic semiconductor and the Fermi level of the metal increases. This naturally affects the nature of charge injection, making the contact resistances between the metal and the polymer nonlinear at low impurity concentrations. Self-assembly of SAMs on Au surfaces proved to be a more effective way of controlling injection barriers between the metal and the polymer. This technique can be used to systematically engineer these energy barriers and carefully study the effect of band alignment on charge injection in transistors. Organic electronic materials and devices constitute a novel and exciting field and show great potential for commercial applications in the near future. Understanding the physics of operation in these devices is just as www.iosrjournals.org
82 | Page
Controlling Charge Injection In Organic Field-Effect Transistors Using Self-Assembled Monolayers rewarding as developing new materials and device designs. In fact, this understanding is essential for the progress of the field and the application of these devices. The primary goal of this thesis has been precisely this: To contribute and enhance our understanding of the nature of charge transport in organic electronic devices. The results of our experiments have placed us among important contributors to this field and this work will continue along new directions in the future.
References                       
Watkins, N. J.; Yan, L.; Gao, Y. Appl. Phys. Lett. 2002, 80, 4384-4386. Knupfer, M.; Paasch, G. J. Vac. Sci. Technol. A 2005, 23, 1072-1077. Ishii, H.; Sugiyama, K.; Ito, E.; Seki, K. Adv. Mater. 1999, 11, 605-625. Wan, A.; Hwang, J.; Amy, F.; Kahn, A. Org. Elec. 2005, 6, 47-54. Gao, W.; Kahn, A. Appl. Phys. Lett. 2001, 79, 4040- 4042. Gao, W.; Kahn, A. J. Appl. Phys. 2003, 94, 359-366. Hamadani, B. H.; Ding, H.; Gao, Y.; Natelson, D. Phys. Rev. B 2005, 72, 235302. Hamadani, B. H.; Natelson, D. J. Appl. Phys. 2005, 97, 064508. Campbell, I. H.; Rubin, S.; Zawodzinski, T. A.; Kress, J. D.; Martin, R. L.; Smith, D. L.; Barashkov, N. N.; Ferraris, J. P. Phys. Rev. B 1996, 54, R14321-R14324. N¨uesch, F.; Rotzinger, F.; Si-Ahmed, L.; Zuppiroli, L. Chem. Phys. Lett. 1998, 288, 861-867. Zuppiroli, L.; Si-Ahmed, L.; Kamaras, K.; N¨uesch, F.; Bussac, M.N.; Ades, D.; Siove, A.; Moons, E.; Gr¨atzel, M. Eur. J. Phys. B 1999, 11, 505-512. Tour, J. M.; Rawlett, A. M.; Kozaki, M.; Yao, Y.; Jagessar, R. C.; Dirk, S. M.; Price, D. W.; Reed, M. A.; Zhou, C. -W.; Chen, J.; Wang, W.; Campbell, I. H. Chem. Eur. J. 2001, 7, 5118-5134. Gundlach, D. J.; Jia, L.; Jackson, T. N. IEEE Elec. Dev. Lett. 2001, 22, 571-573. Kim, S. H.; Lee, J. H.; Lim, S. C.; Yang, Y. S.; Zyung, T.; Jpn. J. Appl. Phys. 2003, 43, L60-L62. Pernstich, K. P.; Haas, S.; Oberhoff, D.; Goldmann, C.; Gundlach, D. J.; Batlogg, B.; Rashid, A. N.; Schitter, G. J. Appl. Phys. 2004, 96, 6431-6438.5 Kline, R.J.; McGehee, M.D.; Toney, M.F. Nat. Mater. 2006, 5, 222-228. de Boer, B.; Hadipour, A.; Mandoc, M. M.; vanWoudenbergh, T.; Blom, P. W. M. Adv. Mater. 2005, 17, 621- 625. Hamadani, B. H.; Natelson, D. Appl. Phys. Lett. 2004, 84, 443-445. Cai, L.; Yao, Y.; Yang, J.; Price, D. W., Jr.; Tour, J. M. Chem. Mater. 2002, 14, 2905-2909. Sigma-Aldrich Inc., St. Louis, MO. Hoshino, H.; Yoshida, M.; Uemura, S.; Kodzasa, T.; Takada, N.; Kamata, T.; and Yase, K. J. Appl. Phys. 2004, 95. Surface Potential Detection manual, Veeco Inst. Sec.231.6. Rep, D. B. A.; Morpurgo, A. F.; Klapwijk, T. Org. Elect. 2003, 4, 201-207.
Authors Biography M.K.Madhu is working as lecturer in S.S.S Degree College, Anantapuram. He is having 18 years of teaching experience. He received his M.phil. from periyar university,Tamilnadu in the 2007. He is pursuing Ph.D in Dravidian university.His areas of interests are micro controllers and Embedded systems.
Dr. K. Chandra Sekhara Reddy is working as Associate Professor of Physics in S.S.B.N.College, Anantapur. He is having 25 years of teaching experience. He received his Ph.D. from Sri Krishnadevaraya University, Anantapuram in the year 1996. He guided 12 M.Phil students. Five scholars are working under his guidance for their Ph.D. He published 13 papers in National and International Journals. His areas of interest are Liquid Crystals, Nano materials and Embedded systems.
83 | Page